AuCd4: A Hume-Rothery Phase with VEC of 1.8 and Icosahedral and Trigonal-Prismatic Clusters as Building Blocks.
Jana, Partha P.; Lidin, Sven; Inorganic chemistry 54 (2015) 713–721; doi:10.1021/ic500616t

data_4339977
_publ_section_title
;
 AuCd4: A Hume-Rothery Phase with VEC of 1.8 and Icosahedral and
 Trigonal-Prismatic Clusters as Building Blocks.
;
_journal_issue                   3
_journal_name_full               'Inorganic chemistry'
_journal_page_first              713
_journal_page_last               721
_journal_paper_doi               10.1021/ic500616t
_journal_volume                  54
_journal_year                    2015
_chemical_formula_sum            'Au0.987 Cd4.07'
_chemical_formula_weight         651.9
_space_group_IT_number           176
_symmetry_cell_setting           hexagonal
_symmetry_Int_Tables_number      176
_symmetry_space_group_name_Hall  '-P 6c'
_symmetry_space_group_name_H-M   'P 63/m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            54
_cell_length_a                   21.3259(14)
_cell_length_b                   21.3259(14)
_cell_length_c                   14.1254(9)
_cell_measurement_reflns_used    2791
_cell_measurement_temperature    293
_cell_measurement_theta_max      30.82
_cell_measurement_theta_min      3.08
_cell_volume                     5563.5(6)
_computing_cell_refinement
;
CrysAlisPro, Agilent Technologies,
Version 1.171.35.21 (release 20-01-2012 CrysAlis171 .NET)
(compiled Jan 23 2012,18:06:46)
;
_computing_data_collection
;
CrysAlisPro, Agilent Technologies,
Version 1.171.35.21 (release 20-01-2012 CrysAlis171 .NET)
(compiled Jan 23 2012,18:06:46)
;
_computing_data_reduction
;
CrysAlisPro, Agilent Technologies,
Version 1.171.35.21 (release 20-01-2012 CrysAlis171 .NET)
(compiled Jan 23 2012,18:06:46)
;
_diffrn_ambient_temperature      293
_diffrn_detector_area_resol_mean 16.1367
_diffrn_measured_fraction_theta_full 0.98
_diffrn_measured_fraction_theta_max 0.91
_diffrn_measurement_device       'four-cycle diffractometer'
_diffrn_measurement_device_type  'Xcalibur, Eos'
_diffrn_measurement_method       '\p scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_source         'Enhance (Mo) X-ray Source'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.7107
_diffrn_reflns_av_R_equivalents  0.0644
_diffrn_reflns_av_sigmaI/netI    0.0672
_diffrn_reflns_limit_h_max       29
_diffrn_reflns_limit_h_min       -25
_diffrn_reflns_limit_k_max       30
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            18155
_diffrn_reflns_theta_full        29.44
_diffrn_reflns_theta_max         30.89
_diffrn_reflns_theta_min         3.09
_exptl_absorpt_coefficient_mu    55.43
_exptl_absorpt_correction_T_max  1
_exptl_absorpt_correction_T_min  0.52
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro, Agilent Technologies,
Version 1.171.35.21 (release 20-01-2012 CrysAlis171 .NET)
(compiled Jan 23 2012,18:06:46)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            'silvery with metallic luster'
_exptl_crystal_density_diffrn    10.5038
_exptl_crystal_F_000             14760
_exptl_crystal_size_max          0.06
_exptl_crystal_size_mid          0.04
_exptl_crystal_size_min          0.02
_refine_diff_density_max         4.21
_refine_diff_density_min         -3.95
_refine_ls_extinction_coef       657(15)
_refine_ls_extinction_method
'B-C type 1 Gaussian isotropic (Becker & Coppens, 1974)'
_refine_ls_goodness_of_fit_gt    1.14
_refine_ls_goodness_of_fit_ref   1.09
_refine_ls_number_constraints    12
_refine_ls_number_parameters     243
_refine_ls_number_reflns         5544
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0982
_refine_ls_R_factor_gt           0.0435
_refine_ls_shift/su_max          0.0132
_refine_ls_shift/su_mean         0.0013
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     w=1/(\s^2^(I)+0.0004I^2^)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.0769
_refine_ls_wR_factor_ref         0.0980
_reflns_number_gt                3184
_reflns_number_total             5544
_reflns_threshold_expression     I>3\s(I)
_cod_data_source_file            ic500616t_si_002.cif
_cod_data_source_block           I
_cod_depositor_comments
;
The following automatic conversions were performed:

'_diffrn_radiation_probe' value 'X-ray' changed to 'x-ray' according
to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2281 2013-09-26 08:29:07Z andrius 

 Adding full bibliography for 4339977--4339978.cif.

The following automatic conversions were performed:

data name '_atom_site_site_symmetry_mutiplicity' was replaced with
'_atom_site_site_symmetry_multiplicity' as specified in the
replacement file 'data/replacement-values/replacement_tags.lst'.

Automatic conversion script
Id: cif_correct_tags 9268 2022-04-12 08:56:07Z antanas 
;
_cod_database_code               4339977